Structural Behaviour of Laterally Loaded
Plain and Fibre Reinforced Precast Foamed
Concrete Sandwich Panels
Surya Bose 1, Meera C.M 2
M. Tech. Student, Department of Civil Engineering, Sree Narayana Gurukulam College of Engineering , Ernakulam,
Assistant Professor, Department of Civil Engineering, Sree Narayana Gurukulam College of Engineering , Ernakulam,
Kerala , India2
ABSTRACT: Foamed concrete is an aerated lightweight concrete. Foamed concrete does not contain coarse aggregate. Foamed concrete can be designed to have any density of range 400-1850 kg/m3.Experimental studies were carried out to investigate the structural behaviour of precast foamed concrete sandwich panels under lateral load. Mechanical properties of both plain and coir fibre reinforced foamed concrete were obtained, which are needed for the design of sandwich panel. It is found that the fibre reinforcement largely enhances the mechanical behaviour of foamed concrete.
KEYWORDS: Foamed concrete, Light weight concrete, Compressive strength, coir fibre, Ultimate load carrying capacity.
II. RELATED WORK
E.A. Flores Johnson,Q.M Li “Structural behaviour of composite sandwich panels with plain and fibre-reinforced foamed concrete cores and corrugated steel faces” (2012) studied the four-point bending response and failure mechanisms of sandwich panels with corrugated steel faces and either plain or fibre-reinforced foamed concrete core. Mechanical properties of both plain and polyvinyl alcohol fibre-reinforced foamed concrete were obtained, which are needed for the design of sandwich panel and numerical modelling. It was found that the fibre-reinforcement largely enhances the mechanical behaviour of foamed concrete and composite sandwich panels. Vinoth Kumar, Kavitha, “Experimental Study on Composite Sandwich Panels with Concrete and Corrugated Steel Faces” (2016) conducted experimental investigation on composite sandwich panel. Sandwich composite panel consists of three layers of two different materials (Concrete and steel). Concrete was sandwiched between steel layers (i.e a 1 mm thick plain cold-rolled sheet on top and corrugated sheet underneath concrete layer). Panel dimension is of 650mm wide, 100mm high and 1250mm long (One Way Distribution). Six numbers of panels were casted of which three from each Reinforced concrete panel and Composite Sandwich panel. Embossment of seven numbers was provided in corrugation and 10mm diameter eight number of shear stud required to connect plain Cold Rolled sheet and corrugation layer. Behaviour of sandwich panel as well as RC Panel was tested under Four-point loading setup. Test results and failure pattern of both panels were compared with one another. M.A. Othuman Mydin, N.A. Rozlan, S. Ganesan, “Experimental Study on the Mechanical Properties of Coconut Fibre Reinforced Lightweight Foamed Concrete” (2015),conducted experimental studies on the use of coir fibre for the enhancement of mechanical properties of foamed concrete which focuses on 3 parameters which are compressive strength, flexural strength and splitt tensile strength with different percentages of coconut fibre (0%, 0.2% and 0.4%). The addition of coconut fibre significantly improved all the properties investigated. The results of the test showed that the compressive strength, flexural strength and splitting tensile strength of the foamed concrete increase as the fibre volume percentage of the coconut coir fibre increased in the concrete mix.
The compressive strength of foam concrete with different percentages of coir fibre (0%, 0.2%, 0.4%, 0.6%, 0.8%) was determined at the age of 28 days using 150 mm x 150 mm x 150 mm concrete cubes in accordance with IS 516-1959. Plain and coir fibre reinforced foamed concrete mix were prepared by foam generator. Then the concrete is filled in the mould. After 24hrs of moist air curing, specimens were placed in water tank for water curing of 28 days. Specimens of 150 mm x 150 mm x 150 mm foam concrete cubes were tested in a Compression Testing Machine (CTM) of capacity 2000 kN. The bearing surfaces of testing machine was wiped clean and any loose sand or other material was removed from the surface of the specimen which are to be in contact with the compression platens. The load was applied without shock and increased continuously at a rate of approximately 140 kg/cm2/min until the resistance of the specimen to the increasing load breaks down and no greater load can be sustained. The maximum load applied to the specimen was then recorded. The compressive strength of the specimen was calculated by dividing the maximum load applied to the specimen during the test by the cross-sectional area.
Fig 2: Compressive strength with Percentage of coir fibre
From the test results it can be seen that when the coir fibres added to the foam concrete mix the compressive strength increases slightly. The optimum value obtained is 15.3 N/mm2 by addition of 0.4% of coir fibres by weight of the cement content. Beyond 0.4% the strength value is found to be decreasing. Increase in compressive strength is due to the crack arresting properties of the fibres.
The flexural behaviour of the plain, coir fibre reinforced and normal concrete panels were analysed .The clear span is 1400mm.The load is applied at the midspan of the panel.
12.5 13 13.5 14 14.5 15 15.5
0% 0.20% 0.40% 0.60% 0.80%
Percentage of coir fibre
Fig 3: Bending test of the Panel Fig 4: Corrugated steel sheet with holes
The sandwich panels were manufactured in using 0.7 mm thick corrugated steel sheets with holes as core and foam concrete as faces. Foamed concrete was prepared and cast into the mould .The panels of normal concrete (M 20), plane foam concrete and fibre reinforced foam concrete (0.4%) were cast. The support provided at both the ends and the load is applied at the mid span. Two dial gauges were fitted at both the sides and from the values obtained load deflection graph is plotted. The panels of 1600mm length, 720mm width and 110mm thickness were used for the experiment.
Fig.5 shows the load deflection graph of plain foam concrete, fibre reinforced foam concrete and of normal concrete panel. All the panels are of size 1600mm length ,720 mm width and 110mm thickness.
0 5 10 15 20 25 30 35
0 5 10 15 20
normal concrete the ultimate load obtained is 33.12 kN. There is a significant increase in the flexural strength when the foam concrete is reinforced with coir fibre. There is a 30% increase in the flexural strength of the foam concrete panel when it is reinforced with coir fibre. Even if the flexural strength of fibre reinforced foam concrete panel (FRFCP) is lesser than the concrete panel, when considering the lightweight nature and reduced cost, FRFCP is a better option.
The findings of experimental investigations on the potential of coir fibre in lightweight foamed concrete for the flexural strength improvement are reported in this study. The addition of coir fibre improved the strength of the foamed concrete significantly. Since the use of coir fibres has given an excellent result, there is still possibility of the invention of new products containing coir fibres with improved results.
 Ameer A. Hilal, Nicholas H. Thom, and Andrew R. Dawson “The Use of Additives to Enhance Properties of Pre-Formed Foamed Concrete”,
International Journal of Engineering and Technology,Vol.7,No.4pp.286-293,2009.
 Ashish S. Moon1, Dr. Valsson Varghese“Sustainable Construction With Foam Concrete As A Green Green Building Material”,International
Journal of Modern Trends in Engineeringand Research,Vol.3,Issue 02,2015 .
 Ashish S. Moon1, Dr. Valsson Varghese, S.S. Waghmare “Foam Concrete Can be used for Sustainable construction as a Building
Material” ,International Journal of Modern Trends in Engineeringand Research ,Vol.3,Issue02,pp.1428-1431,2015 .
 E.A. Flores Johnson,Q.M Li “Structural behaviour of composite sandwich panels with plain and fibre-reinforced foamed concrete cores and
corrugated steel faces”, Composite Structures,Vol. 94,pp.1555–1563,2012
 Fengtao Bai , James S. Davidson“Analysis of partially composite foam insulated concrete sandwich structures”, Engineering
Structures ,Vol.91,pp. 197–209,2015
 Hanizam Awang, Muhammad Hafiz Ahmad, “Durability Properties of Foamed Concrete with Fiber Inclusion”, International Journal of Civil,
Environmental, Structural, Construction and Architectural Engineering Vol.8,No.2,pp.273-276,2014
 K. Krishna Bhavani Siram,K. Arjun Raj, “Concrete + Green=Foam concrete”,International Journal of Civil Engineering And
 Maheshkumar H Tharkrele, “ Experimental study on foam concrete,“International Journal of Civil,Structural,Environmental and Infrastructure
 M.A. Othuman Mydin, N.A. Rozlan, S. Ganesan, “Experimental Study on the Mechanical Properties of Coconut Fibre Reinforced Lightweight
 Vinoth Kumar , Kavitha , “Experimental Study on Composite Sandwich Panels with Concrete and Corrugated Steel Faces,“International
Journal for Scientific Research & Development ,Vol. 4,pp.939-942,2016.
 Shankar Ganesan, Md Azree Othuman Mydin, Mohd Yazid Mohd Yunos,“Foam Resistance Performance of coir fibre reinforced foamed
concrete wall panel”,Advances in Environmental Biology, Vol.9,Issue.4,pp.117-120,2015.
 Y.H. Mugahed Amran , A.A. Abang Ali, Raizal S.M. Rashid, Farzad Hejazi, Nor Azizi Safiee, “Structural behavior of axially loaded precast
foamed concrete sandwichpanels”, Construction and Building Materials ,Vol.107 ,pp. 307–320,2016 .
 Y.H. Mugahed Amran , A.A. Abang Ali, Raizal S.M. Rashid, Farzad Heja , NorAzizi Safiee, “Structural behavior of laterally loaded precast